Structures of Ta3As and (Nb,Ta)3As
Post on 21-Sep-2016
Te(OH)6.2(NH4)2HPO 4 ET Te(OH) 6. Na2HPO 4. H20 1447
poss6de un voisinage constitu6 par six atomes d'oxy- g6ne appartenant ~t trois octa6dres TeO 6 et par la mol6cule d'eau O(w).
L'atome Na(2) est entour6 seulement de six atomes d'oxyg6ne, provenant par moiti6 des octa6dres TeO 6 et des t&ra6dres PO 4.
Le Tableau 6 donne les principales distances inter- atomiques et angles de liaison.
La pr6sence d'une mol6cule d'eau sur un axe ternaire pose un probl6me en ce qui concerne une localisation ~ventuelle des protons de cette molecule. La pr6sence/L proximit~ de cette derni~re de groupements HPO 4 sugg~re la possibilit~ de l'existence d'un groupement hydronium H3 O+. Dans cette hypoth~se, les trois atomes d'oxyg6ne O(1) distants de 2,64 /k de cette mol6cule d'eau seraient reli6s/t cette derni6re par deux
liaisons hydrog6ne provenant des protons de la mol6cule d'eau, la derni6re liaison &ant assur6e par le proton du groupement HPO 4. Un essai de localisation des protons par minimisation d'6nergie (Tordjman, 1979) conduit/t leur attribuer une position g6n6rale 6(c) en x = 0,186, y = 0,682, z = 0,277. Dans cette configuration, on observe les distances suivantes: H - O(w) = 0,96, H--O(1) = 1,70 /k, avec des angles O(1)-H--O(w) = 167 et H--O(w)-H = 112 . Une &ude par diffraction de neutrons est envisag6e pour v6rifier cette hypoth6se.
R6f6renees PREWITT, C. T. (1966). SFLS5. A Fortran IV Full-Matrix
Crystallographic Least-Squares Program. TORDJMAN, I. (1979). J. Appl. Cryst. 12. A paraJtre.
Acta Cryst. (1979). B35, 1447-1450
Structures of Ta3As and (Nb,Ta)3As*
BY Yu WANG, L. D. CALVERT,~" E. J. GABE AND J. B. TAYLOR Chemistry Division, National Research Council of Canada, Ottawa K1A 0R9, Canada
(Received 11 October 1978; accepted 23 February 1979)
Abstract. Ta3As (a new structure type), monoclinic, B2/b, a = 14.6773(6), b = 14.5505(4), c = 5.0954 (2) /k, 3' = 90.572 (3) , Z = 16; a full-matrix least-squares refinement gave R = 0.081 for 2440 observed hkl, using graphite-monochromated Mo radiation (;ta t = 0. 70932 /k). One (Nb,Ta)3As crystal, P42/n, a = 10.308 (1), c = 5.148 (1)/k, Z = 8, had the Ti3P-type structure; a refinement on a twin-type model gave R = 0.072 for 3709 observed hkl. Both structures contain [AsM~0] bicapped square antiprism units with average interatomic distances for Ta3As and (Nb,Ta)3As of M--M = 3.12 and 3.13 /k, M-As = 2.74 and 2.74 /k and As -As = 3.87 and 3.92 /k respectively. TaaAs is an ordered variant of NbaAs.
Introduction. Ta3As and Nb3As were reported to have the Ti3P structure by Ganglberger, Nowotny & Benesovsky (1966). This was confirmed for Nb3As by Rundqvist, Carlsson & Pontchour (1969) but they suggested the Fe3P or a-V3S structure for Ta3As and, in addition, found some of the lines in Ta3As powder patterns split or broadened, but were unable to obtain single crystals. Ta3As was characterized as monoclinic with a new structure type by Murray, Taylor, Calvert, Wang, Gabe & Despault (1976) on the basis of powder
* NRCC No. 17332. t To whom correspondence should be addressed.
patterns and single-crystal precession photographs. Their powder patterns were not identical for all samples and their single crystals were twinned or of poor quality. Single-crystal studies were undertaken in an attempt to clarify these discrepancies. Many apparently good single crystals grown by iodide transport in tantalum crucibles (Murray et al., 1976) were examined by Laue photographs and found to be twinned, i.e. Laue ellipses were doubled. The first good crystal found was mounted on a four-circle computer-controlled diffractometer. The symmetry was found to be te- tragonal, not monoclinic as expected, with reflection conditions 00/, l = 2n and hk0, h + k = 2n and a c axis of 5.148 /k, intermediate between those of TaaAs (5.0954 /k) and Nb3As (5.189 /k; Waterstrat, Yvon, Flack & Parth6, 1975). Cell parameters were obtained by centring reflections with 8 > 60 (Table 1). The Ta used in preparing these specimens was later found to have contained -..1% Nb. Intensities were measured (Table 1) using local programs (for details see Wang, Gabe, Calvert & Taylor, 1976a) and corrected for Lorentz, polarization and absorption effects. Because the composition was not certain the absorption coefficient was an experimental value. Intensities were measured at 10 intervals as the crystal was rotated around the diffraction vector (0 < ~, < 180 ) for several reflections and the appropriate absorption corrections were calculated with different values of/h.
1979 International Union of Crystallography
1448 TaaAs AND
The value which gave the best fit was chosen. This corresponded to Nb2TaAs, a composition consistent with the results of the structure refinement. The structure was solved by direct methods. Refinement by full-matrix least squares with allowance for anomalous dispersion converged to R t = ~, IAFI/~ IFol = 0.16 with Nb scattering factors used for all metal-atom sites but occupancies refined with the scale held constant. Two sites, M(1) and M(3), were later changed to Ta scattering factors. Careful inspection showed that the agreement for the 344 observed hhl and hOl reflections was better (R~ = 0.09) than for the hkl ones. A disordered model, derived by a 180 rotation around (1 i0), did not refine successfully. A 'twin' model was successfully refined on structure factors defined as F 2 = F 2 + tF 2 where F~ is calculated from x,y,z for the normal structure and F 2 from y ,x , - z for the twin fragment, and t is the ratio of twin present and is refined as a parameter. This model refined to R~ = 0.072 with t = 0.225 for the 3709 observed hkl. Occupancies for two sites [M(1) and M(3)] were 0.70 and 0.67 of Ta respectively and these are therefore believed to be mixed Ta and Nb sites. At this stage a difference map, computed for 'twin-free' F o, showed residual features on the two sites [M(2) and As] which interchange metal for As after the twin operation. These residual features were removed by adding 0.12 Nb in the M(2)
Table 1. Structure refinement details
Ta3As (Ta,Nb)3As Crystal size (mm) 0.05 x 0-10 x 0.13 0.03 x 0-05 x 0.12 gt (mm-l) 138.5 62.3 Transmission factors 0.0025-0.0518 0.06-0.19 Scan range() 0.5 + 0.7 tan 0+ 0.5 0.5 + 0.7 tan 0+ 0-7 2 Omax 75 o 120 o Measurements 2888 x 2 4429 Observed, I > 20 2440 3709 Reflections used 50 32
for cell parameters
'twin' site and 0.11 As in the As 'twin' site. The final parameters (corresponding to F~) are given in Table 2. This approximates Nb2TaAs but in view of the uncertain absorption correction and the refinement problems, the composition must be considered as tentative. Although this model refined successfully there may be other equally valid models. An attempt at obtaining a microprobe analysis for this crystal failed because the crystal was lost during polishing. However, a previous X-ray fluorescence analysis on this crystal had confirmed the presence of Nb. It seems clear from the structure derived, the values of the cell parameters and the intermediate powder patterns observed (Mur- ray et al., 1976) that Nb3As can dissolve some TaaAs without change of structure.
A continued search produced a monoclinic crystal of Ta3As. Lattice parameters were in good agreement with those of Murray et al. (1976) for Ta3As and two sets of data were measured for this crystal and averaged (Table 1). A trial based on a 45 rotation of the (Nb,Ta)aAs structure with two Ta3As in the asym- metric unit did not refine. A refinement of x,y coordinates only, based on the 168 hk0 reflections, converged (R 1 = 0.11); z coordinates were then added and a difference map showed that atoms corre- sponding to M(2) and As of the NbsAs structure were shifted by c/2 relative to the trial structure (Fig. 1). Full-matrix refinement with anisotropic thermal param- eters and allowance for anomalous dispersion and isotropic extinction converged to R~ = 0.081 for 2440 hkl (I > 20). A difference Fourier map showed no significant residual features other than small irregular residuals near the Ta sites, probably attributable to inadequacies in the absorption corrections. Consider- able pains were taken to define the shape of the crystal and check the calculated transmission factors by azimuthal scans around the diffraction vector; these checks were satisfactory. Refinement of the data without absorption corrections converged to R 1 = 0.18
M(1) M(2) M(3) As *M(2') *As'
Table 2. Atomic parameters for (Nb,Ta)aAs
The temperature factor was of the form exp [-8zr 2 U (sin 0/2)2].
0.703 (4) 1.007 (7) 0.673 (4) 0.783 (8) 0.119 (8) 0.114 (10)
Scattering factor used x y z U (A 2)
Ta 0.15544 (5) 0.66315 (5) 0.23449 (11) 0.0043 (1) Nb -0.10159 (7) 0.75909 (7) 0.48680 (16) 0.0017 (1) Ta -0.03971 (6) 0.44440 (6) 0.25573 (11) 0.0043 (1) As --0.23299 (12) 0-54330 (12) 0.51476 (26) 0-0039 (2) Nb -0.2594 (8) -0.1032 (8) 0.484 (2) 0.006 (11) As 0.538 (2) -0.263 (2) 0.505 (4) 0.020 (3)
[t = 0.225 (4)1
* No twin component in the refinement.
Ta3As AND (Nb,Ta)3As 1449
~ [1 m
/ . . . . . . .
with negative isotropic temperature factors. The final positional parameters are given in Table 3.*
Diseusslon. The intermediate (Nb,Ta)aAs structure (Fig. la) is of the TiaP type which has been discussed by Nawapong (1966), Chen& Franzen (1972) and Waterstrat (1975) and thus needs no detailed descrip- tion here. Lundstr6m & Snell (1967) described the As coordination as tricapped trigonal prismatic (CN = 9) but this was modified by Waterstrat (1975) to a bicapped square antiprism description (CN = 10). The Ta3As structure (Fig. lb) contains open columns of octagonal antiprisms of Ta atoms at z = ~ and forming 382 + 3282 (1:1) networks. These are centred by [Ta2As 2] diamonds at z = 0 and which form 44+ 44 (1:1) nets. In both structures As has 10 Ta neighbours (both averages = 2.77 /t,); Ta(1) and Ta(11) are coordinated to 12 Ta (both averages = 3.10 /~) plus 2 As (both averages = 2.63 /~,) while Ta(2), (22), (3) and (33) have 11 Ta [overall averages 3.15 and 3.14 /~ for (Nb,Ta)3As and Ta3As respectively] plus 4 As neighbours at both 2.64 and 2.98/~, in both cases. The coordinations in Nb3As, (Nb,Ta)aAs and Ta3As are compared in Table 4 in detail.*
The 'twin' mechanism for (Nb,Ta)3As leaves the atomic distribution on the planes z = ~, ] unchanged but interchanges metal and As atoms at z = 0, (Wang, Gabe, Calvert & Taylor, 1976b). The basic unit
* Lists of structure factors for Ta3As and (Nb,Ta)3As, aniso- tropic thermal parameters for Ta3As, and Table 4 have been deposited with the British Library Lending Division as Supplemen- tary Publication No. SUP 34288 (57 pp.). Copies may be obtained through The Executive Secretary, International Union of Crystallography, 5 Abbey Square, Chester CH 1 2HU, England.
Fig. 1. The ~001) projections of (a) the tetragonal MaAs structure (TiaP type) and (b) the monoclinic TaaAs structure. Corre- sponding sets of symmetry elements are marked in both cells; symmetry centres are marked by Q. Corresponding sets of metal sites are numbered as in Tables 2 and 3.
Table 3. Positionalparameters (x 104) of Ta3As
x y z
Ta(l)* -2531 (1) 4087 (1) 2283 (2) Ta(11) -1584 (1) --41 (1) 2541 (2) Ta(2) --667 (1) 1715 (1) 5002 (2) Ta(22) --745 (1) 3215 (1) --115 (2) Ta(3) --2423 (1) 2025 (1) 2533 (2) Ta(33) --484 (1) --60 (1) 7509 (2) As(l) -3862 (2) 1553 (2) --146 (6) As(11) --999 (2) 1402 (2) -12 (6)
* Atoms are numbered for comparison with the Ti3P-type structure of N b 3As: Ta(1) and Ta(11) correspond to N b(1).
Fig. 2. A perspective view of the fourfold [AsTa~0] grouping, which is centred on a centre of inversion (marked by both here and in Fig. lb). The As atoms are omitted from the [AsTa~0] groups.
1450 TaaAs AND (Nb,Ta)aAs
in both NbaAs and TaaAs is the [AsM~0] bicapped square antiprism. In TaaAs four such units surround a centre of inversion (Fig. 2), sharing two edges and two triangular faces. In Nb3As these centres become 42 axes. Consequently the columns of [Ta2As2] diamonds are displaced by c/2 in alternate octagonal columns in TaaAs (Fig. lb), whereas in Nb3As (Fig. la) the [Nb2As2] diamonds are all at the same height and the [AsMlo] units share two edges and two corners.
A similar displacement of alternate columns is found between the structures of a-VaS and fl-VaS (Pedersen & Gronvold, 1959) which contain columns of octagonal antiprisms, centred by [M2S 2] diamonds, arranged in a more symmetric manner. NiaP (Aronsson, 1955) is analogous to tq-V3S and Ta3As.
The twinning mechanism found in the refinement of (Nb,Ta)3As provides a possible explanation for the variability of powder patterns and the difficulties of obtaining good single crystals reported by Rundqvist, Carlsson & Pontchour (1969) and Murray et al. (1976) as Nb is a frequent contaminant in Ta.
The authors would like to thank Dr S. Berman for the X-ray fluorescence analysis.
References ARONSSON, B. (1955). Acta Chem. Scand. 9, 137-140. CHEN, H.-Y. & FRANZEN, F. (1972). Natl Bur. Stand. (US)
Spec. Publ. 364, pp. 651-662. GANGLBERGER, E., NOWOTNY, H. & BENESOVSKY, F.
(1966). Monatsh. Chem. 97, 1696-1697. LUNDSTR6M, T. & SNELL, P.-O. (1967). Acta Chem. Scand.
21, 1343-1352. MURRAY, J. J., TAYLOR, J. B., CALVERT, L. D., WANG, Y.,
GABE, E. J. & DESPAULT, J. G. (1976). J. Less-Common Met. 46, 311-320.
NAWAPONG, P. C. (1966). Acta Chem. Scand. 20, 2737- 274 I.
PEDERSEN, B. & GRONVOLD, F. (1959). Acta Cryst. 12, 1022-1027.
RUNDQVIST, S., CARLSSON, B. & PONTCHOtJR, C.-O. (1969). Aeta Chem. Scand. 23, 2188-2190.
WANG, Y., GABE, E. J., CALVERT, L. D. & TAYLOR, J. B. (1976a). Acta Cryst. B32, 1440-1445.
WANG, Y., GABE, E. J., CALVERT, L. D. & TAYLOR, J. B. (1976b). Abstract PB8. Am. Crystallogr. Assoc. Meeting, Evanston, August, p. 63.
WATERSTRAT, R. M. (1975). J. Less-Common Met. 43, 105- 115.
WATERSTRAT, R. M., YVON, K., FLACK, H. D. & PARTHt~, E. (1975). Acta Cryst. B31, 2765-2769.
Acta Cryst. (1979). B35, 1450-1452
III V Structure du Pyrochlore, TIo.slSbo.71Sb 2 06,32
PAR Y. PIFFARD ET M. TOURNOUX
Laboratoire de Chimie des Solides,* UER de Chimie, 2 rue de la Houssini~re, 44072 Nantes CEDEX, France
(Regu le 13 juillet 1978, accept6 le 5 mars 1979)
Abstract. Tlo.5~Sb~I.~lSbVO6 32, cubic, Fd3m, a - - c= 10-3127 (4) A,'Dm = 6:479 (5)Mg m-3, Z --8~)~ ray data were collected on a three-circle diffractometer. The final unweighted R was 0.037 for 186 independent
xli v Sb m reflexions. As in Ko.51Sb0.67Sb206.26 , the ions are located in a 96(g) position.
Introduction, Nous avons r6cemment d6crit la structure III V du pyrochlore K0.51Sb0,67Sb206,26 dans laquelle l'anti-
moine(III) occupe au sein des tunnels communicants, d+limit6s par la charpente Sb206, une position 96(g) (Piffard, Dion & Tournoux, 1978). C'est la premiere fois qu'il &ait d+montr6 qu'un cation, dans ce type structural, pouvait occuper une position ext+rieure l'axe [ 111 ]. Une phase de ce type, dans laquelle l'alcalin est remplac6 par le thallium(l), a &6 obtenue h l'6tat de poudre microcristalline par B ouchama ( 1973).
* Laboratoire associ6 au CNRS n 279.
Nous avons obtenu des monocristaux de ce pyro- chlore par chauffage/~ l'air pendant 3 h fi 1273 K d'un m6lange d'oxyde thallique et de SbzO a dans un rapport molaire initial T12Oa/Sb20 a de 0,25. La valeur +lev6e de la temperature de preparation entraine des pertes en thallium par volatilit6 et rend peu probable la presence de thallium(III) dans les cristaux obtenus. Les cristaux se pr6sentent sous forme d'octa6dres r6guliers de couleur orange. Leur composition a 6t6 d&ermin6e par diff6rentes techniques: analyse fi la microsonde de CASTAING du monocristal ayant servi fi l'&ude structurale, dosage par spectrophotom&rie d'ab- sorption du thallium et de l'antimoine, &ude M6ssbauer et d&ermination tr6s pr6cise de la densit6 /~ partir de cristaux. L'&ude M6ssbauer montre la pr6sence d'anti- moine(III) mais ne permet pas une d&ermination pr6cise du rapport Sbm/Sb v car l'antimoine(III) est beaucoup moins fortement li6 que rantimoine(V) et pr+sente un environnement tr+s irr6gulier. La presence
1979 International Union of Crystallography